• Study Resource
• Explore

Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Transcript
```PRL 112, 034301 (2014)
week ending
24 JANUARY 2014
PHYSICAL REVIEW LETTERS
Ï
FIG. 2 (color online). Schematics of wave propagation direction with respect to interfacial layers.
FIG. 1 (color online). Schematics of undeformed and deformed
periodic multilayered structures with interfacial phase volume
fractions (a) cÃ°iÃ Â¼ 0.02 and (b) 0.04. (c) Dependence of stress
vs strain and wrinkle amplitude vs strain. The stress-strain results
are given by the continuous black (cÃ°iÃ Â¼ 0.04) and red curves
(cÃ°iÃ Â¼ 0.02); the dashed curve is the solution for flat layers,
assuming no wrinkling. The dotted curves represent the evolution
of the normalized wrinkle amplitude (right axis). The stiffness
ratio of the phases is Î¼Ã°iÃ =Î¼Ã°mÃ Â¼ 100.
Here, we analyze the propagation of elastic waves in
finitely deformed periodic materials. To this end, we consider incremental small-amplitude motions superimposed
on a finitely deformed state [20]. Differently from a plane
wave, a wave propagating in a periodic structure is the
superposition of plane waves, which can be described
by the Bloch function [1,23]. Consequently, the smallamplitude motions are implemented in terms of Bloch
waves ui Ã°x; tÃ Â¼ Ui Ã°x; tÃ expÃ°ik Â· xÃ, where ui is the
displacement, k is the Bloch vector and Ui is a periodic
function subjected to the periodicity condition U i Ã°x; tÃ Â¼
Ui Ã°x Ã¾ a; tÃ with a being a lattice translation vector
[12,20,23]. To perform this analysis, we use the finite
element method, which allows us (i) to obtain the solution
for the deformed periodic composite after the bifurcation,
and (ii) then superimpose the Bloch-Floquet periodicity
condition on the deformed state and solve the eigenvalue
problem associated with the wave equations. For completeness, the numerical solution was verified against exact
analytical solutions for finitely deformed infinite homogeneous and layered materials, and excellent agreement
was found. We define the direction of wave propagation
via angle Ï as shown in Fig. 2.
The influence of interface wrinkling on wave propagation is shown in Fig. 3 which compares the dispersion
diagrams for (a) the undeformed state, where the applied
strain Ïµ Â¼ 0, to (b) those at the onset of wrinkling formation
Ïµ â Ïµcr , and to (c) those for a developed wrinkled state
Ïµ > Ïµcr . Figure 3 shows examples of dispersion diagrams
for various composites with different stiffness ratios
rÎ¼ Â¼ Î¼Ã°iÃ =Î¼Ã°mÃ : different density contrast ratios rÏ Â¼
ÏÃ°iÃ =ÏÃ°mÃ , and different interfacial layer volume fractions
of cÃ°iÃ to allow comparison
pï¬ï¬ï¬ï¬ï¬ï¬ï¬ï¬ï¬ï¬ï¬ï¬ï¬of these effects. The normalized
frequency Ï~ Â¼ Ïh ÏÃ°mÃ =Î¼Ì is reported. The dispersion diagram of the undeformed structure appears in the top row.
The composites present in columns (1)â(3) and (4) exhibit
elastic instabilities at different levels of critical strain, in
particular, at Ïµcr Â¼ 0.040 08 and Ïµcr Â¼ 0.0086, respectively. Consequently, we present the dispersion diagrams
for these cases at different strain levels (middle rows),
namely at Ïµ Â¼ 0.04 for composites in columns (1)â(3)
and Ïµ Â¼ 0.01 for column (4). Finally, we show the
dispersion diagrams for a developed wrinkled state in
the bottom row for strains of Ïµ Â¼ 0.048 for composites
in columns (1)â(3), and Ïµ Â¼ 0.017 for column (4). For composites present in columns (1) and (2), the normalized
amplitudes of the wrinkles are A~ Â¼ 0.2687 and 0.5075 at
Ïµ Â¼ 0.04 and 0.048, respectively. The corresponding amplitudes for the composite (3) are 0.271 and 0.524, respectively. For the composite (4), the amplitudes of the
wrinkles are A~ Â¼ 0.522 and 1.058 at Ïµ Â¼ 0.01 and
0.017, respectively.
The dispersion diagrams show different branches of
wave propagation including transverse and longitudinal
waves. In our analysis, we specifically focus on identifying
complete band gaps, when both, longitudinal and transverse waves, cannot propagate. The undeformed composite
does not filter waves in a direction along the interface at any
frequency; however, the deformed composites with
wrinkled interfaces exhibit clear band gaps [see columns
(1), (2), and (4) in line (b)]. The frequency range of the
band gaps is denoted by the grey filled area in Fig. 3.
Note that one-dimensional phononic crystals with flat
layers can never prevent wave propagation parallel to the
layers [24]. In contrast, the wrinkled interfaces introduce
variations of the mechanical properties in the direction
of wave propagation, and, consequently, secondary waves
are generated. The waves interfere with each other such that
for some combination of the material properties,
034301-2
```
Similar